Abstract
Adding impurities or defects destroys crystalline order. Occasionally, however, extraordinary behaviour emerges that cannot be explained by perturbing the ordered state. One example is the Kondo effect, where magnetic impurities in metals drastically alter the temperature dependence of resistivity. In TypeII superconductors, disorder generally works to pin vortices, giving zero resistivity below a critical current j_{c}. However, peaks have been observed in the temperature and field dependences of j_{c}. This peak effect is difficult to explain in terms of an ordered Abrikosov vortex lattice. Here we test the widespread paradigm that an orderdisorder transition of the vortex ensemble drives the peak effect. Using neutron scattering to probe the vortex order in superconducting vanadium, we uncover an orderdisorder transition from a quasilongrangeordered phase to a vortex glass. The peak effect, however, is found to lie at higher fields and temperatures, in a region where thermal fluctuations of individual vortices become significant.
Introduction
It has taken many decades to unravel the effect of weak disorder on the vortex lattice. In the 1970s, investigations initiated by the famous Russian theorist Anatoly Larkin found that any random disorder, no matter how weak, would destroy longrange order^{1}. In Larkin’s perturbative approach^{1,2}, vortex displacements grow linearly with vortex separation r, as measured by the displacement correlation function \(b(r) = \left\langle {\left( {{\bf{u}}_j  {\bf{u}}_l} \right)^2} \right\rangle\), where u_{ j } is the displacement of the jth vortex. This leads to an absence of divergent Bragg peaks. Yet resolutionlimited Bragg peaks from vortex ensembles are clearly observed in scattering experiments^{3,4,5,6}. It turns out the perturbative approach becomes invalid at inplane spacings r = r_{c}, where displacements become larger than ξ, the characteristic scale of the disorder potential. The behaviour at spacings r < r_{c} is accordingly described as belonging to the Larkin or randomforce regime. At larger scales, vortices compete for minima in the disorder potential, slowing the algebraic growth of displacements to b(r) ∝ r^{2ζ}, where the roughness exponent \(\zeta < \frac{1}{2}\). In this socalled random manifold regime, theoretical values for ζ can be derived from the elastic Hamiltonian by scaling estimates^{7,8}, renormalisation group analysis^{9} or variational replicasymmetry breaking techniques^{10,11}. A summary of theoretical values for ζ is reproduced in Table 1.
At larger scales r = r_{A}, where vortex displacements become of order \(a_0 = \left( {2{\mathrm{\Phi }}_0{\mathrm{/}}\sqrt 3 B} \right)^{\frac{1}{2}}\), the lattice spacing set by flux quantisation, the periodicity of the system becomes crucial^{12}. Here the random manifold gives way to a Bragg glass regime. This asymptotic regime at r > r_{A} is characterised by a slower, logarithmic growth^{13} b(r) ∝ ln r and a translational order correlation function \(c_{\mathrm{g}}(r) = \left\langle {{\mathrm{e}}^{{\mathrm{i}}{\bf{g}}.\left( {{\bf{u}}_j  {\bf{u}}_l} \right)}} \right\rangle\) that decays algebraically with an exponent η_{g} (Table 1)^{9,11}. The result is quasilongrange order with algebraically diverging Bragg peaks and so the resulting vortex phase is referred to as the Bragg glass. Note that this term is used to describe both the asymptotic regime and, synecdochically, all three regimes in length scale. Where clarity is called for, we refer to the former as the Bragg glass regime and the latter as the Bragg glass picture.
The Bragg glass picture is expected to break down when dislocations become important. Upon increasing field or disorder strength, a transition to a shortrange ordered vortex glass phase is expected as the pinning energy exceeds the plastic deformation energy^{14,15,16}. Notionally, disorder affects translational order more than orientational order, so the vortex glass is likely hexatic^{17}. The orientational order is characterised by the correlation function \(g_6(r) = \left\langle {{\mathrm{e}}^{{\mathrm{i}}6\left( {\theta _j  \theta _l} \right)}} \right\rangle\), where θ is the nearest neighbour bond angle^{17,18}. Experimentally g_{6}(r) is observed to decay algebraically \(\propto r^{  \eta _6}\) in both the Bragg glass and vortex glass phases. A previous SANS study^{19} of the Bragg glass regime in niobium reported η_{6} = 0.07. In the vortex glass, images of disordered vortex ensembles on the surfaces of NbSe_{2}^{20} and Bi_{2}Sr_{2}CaCu_{2}O_{8+δ}^{21,22} yield η_{6} ≈ 0.06–0.35. These images also show a much faster, exponential decay of translational order, consistent with a hexatic vortex glass.
At temperatures close to the upper critical field B_{c2}(T) at which bulk superconductivity disappears, thermal fluctuations become increasingly important. They drive a proliferation of dislocations and a thermodynamic melting of the vortex lattice. The relative role of thermal fluctuations is quantified by the Ginzburg number^{8} \({\mathrm{Gi}} \approx \left( {\mu _0k_{\mathrm{B}}T_{\mathrm{c}}\kappa ^2{\mathrm{/}}2\xi ^3B_{{\mathrm{c2}}}^2} \right)^2\). The thermal melting line B_{m}(T) of the vortex lattice can be estimated from the phenomenological Lindemann criterion \(\left\langle {u^2} \right\rangle = c_{\mathrm{L}}^2a_0^2\) whereby melting occurs when displacements become a fraction c_{L} of the lattice spacing a_{0}. Typically c_{L} ≈ 0.1–0.2. This gives^{23,24}
where the reduced temperature t = T/T_{c2}. Since Gi ∝ ξ^{−6}, the position of the melting line is strongly dependent on the coherence length ξ. For cuprate superconductors, ξ is a few nanometres, so Gi ≈ 10^{−2}–10^{−3} and the melting line is expected 0.1–10 K (depending on the field) below B_{c2}(T). The expected position of the melting line is confirmed by experiments on the cuprates^{25,26,27}. On the other hand, in lowκ superconductors the melting line is much more difficult to resolve^{5,28} due in part to the smallness of Gi. For our vanadium sample κ = 1.3, ξ = 26 nm (see Methods) and Gi ≈ 6 × 10^{−10}, so B_{m}(T) is anticipated to lie very close to B_{c2}(T). For example, at 0.3 T and with c_{L} = 0.2, B_{m}(T) is within 8 mK of B_{c2}(T).
Equation (1) is obtained with consideration of thermal fluctuations only. A Lindemannlike approach can also be used to predict the field and temperature dependence of the orderdisorder transition line B_{dis}(T) separating the Bragg glass and the vortex glass phases^{23,29,30}. To do this, disorderinduced fluctuations must be considered. At B_{dis}(T) the topologically ordered Bragg glass phase becomes unstable to the formation of dislocations. The dislocation network is anticipated^{16} to appear at scales ≈ r_{A} where displacements are on the order of a_{0}. This can be shown to be equivalent to a generalised Lindemann criterion of the form \(u^2(a_0,0) = c_{\mathrm{L}}^2a_0^2\) where displacements u(r, l) are now parameterised by the separations in and out of the vortex plane^{29,30}. Note that the orderdisorder transition can be driven entirely by disorderinduced displacements. Consequently as thermal fluctuations vanish for T → 0, B_{dis}(0) remains distinct from and less than B_{c2}(0) (Fig. 1), in contrast to the fluctuationinduced melting line B_{m}(T), which curves up to meet B_{c2}(0).
Here we use smallangle neutron scattering (SANS) to probe the longrange correlations of vortex ensembles in a vanadium single crystal. The SANS technique provided the first experimental evidence for the Bragg glass picture: a dependence of the diffracted peak intensity upon magnetic field B that could not be explained by perfect crystalline order^{3}. We also find evidence from the field dependence of the diffracted intensity for a Bragg glass picture at intermediate fields in the phase diagram (Fig. 1). Furthermore we demonstrate the presence of a Bragg glass regime by characterising the shape of the diffraction peak in a highresolution experimental setup (Fig. 2) and using reverse Monte Carlo refinement to extract correlation functions from our data^{19}. Our manuscript proceeds as follows: first we characterise the underlying disorder and the peak effect using magnetometry data on our vanadium single crystal. We subsequently examine our SANS data collected over several experiments and using different experimental setups. These SANS experiments allow the orderdisorder transition to be located. Comparing the orderdisorder transition line B_{dis}(T) determined from SANS with the critical current density j_{c} determined by magnetometry, we discern no jump in j_{c} around B_{dis} in our sample. Instead, we observe a nascent peak effect at fields and temperatures close to B_{c2}(T). This dissimilarity is at odds to the commonly held notion that the peak effect is underpinned by the orderdisorder transition from Bragg glass to vortex glass.
Results
Critical current from magnetometry
Our sample is a vanadium single crystal of cylindrical shape, with length 10 mm and diameter 2R = 5 mm. The [111] cubic crystal direction is coincident with the cylindrical axis. We measured the isothermal magnetisation M as a function of magnetic field H applied parallel to [111], collecting M(H) curves at several temperatures. Figure 3a shows a typical M(H) loop, measured at T = 1.6 K. Extracting the upper critical field from these loops, we find B_{c2}(T) is well described by the empirical relationship^{31} \(B_{{\mathrm{c2}}}(t) = B_{{\mathrm{c2}}}(0)\left( {1  t^2} \right){\mathrm{/}}\left( {1 + \frac{2}{3}t^{7/4}} \right)\) with B_{c2}(0) = 0.440 T. Compared to pure vanadium where T_{c} = 5.47 K^{32}, the small increase in B_{c2}(T) and the small suppression of T_{c} = 5.31 K measured for our sample indicate that the underlying disorder is weak. We obtain a mean free path l = 48 nm (see Methods). From the M(H) loops, the critical current density j_{c} = 3ΔM/2R is calculated using the criticalstate model of Bean^{33}. j_{c} is seen to be small <10^{7} Am^{−2} (c.f. Fig. 3b) compared to the depairing current density \(j_0 \approx H_{\mathrm{c}}{\mathrm{/}}\lambda \approx B_{{\mathrm{c2}}}\)/\(\left( {\sqrt 2 \kappa \lambda } \right) \approx 4 \times 10^{12}\) Am^{−2}, consistent with weak pinning.
Underlying disorder constrains vortex displacements with a pinning force density F_{p} of magnitude j_{c}B. Close to B_{c2}(T), thermal fluctuations enable vortices to ride over the pinning potential and F_{p} is accordingly expected to decrease at high fields and temperatures. It follows that there must be a maximum in F_{p} as a function of B. Many models have been proposed to describe the field dependences of F_{p} and j_{c}. Motivated by data on alloy superconductors with strong pinning, the first models estimated the average pinning force per vortex, accounting semiempirically for the type and geometry of the pins^{34,35,36,37}. For isotropic superconductors like vanadium, these models^{37,38} place the maximum in F_{p}(B) at fields ≥ 0.2B_{c2}. For our vanadium sample we find F_{p}(B) does scale with B_{c2}(T), but the maximum is located at 0.13B_{c2}, i.e. at lower fields than expected and the observed j_{c}(B) dependence is not accurately reproduced by these semiempirical models^{34,35,36,37}.
More recent models for j_{c}(B) consider the contribution to pinning at different length scales^{8} and the dynamic effects of flux creep^{39}. These models give various j_{c} behaviours depending on the regime of field and temperature. For example, the large bundle pinning regime is entered when pinning is weak and vortex length scales are large compared to the penetration depth λ. Here nonlocality of the elastic constants can be neglected. In our lowκ superconductor, λ ≈ 35 nm is short. The minimum vortex lattice spacing a_{0} is 74 nm, the value at B_{c2}(0), so vortex lattice length scales generally exceed λ and we expect to be in the large bundle regime in most of the mixed state. In this regime, j_{c} is theoretically predicted to follow^{8}
where l_{c} is the scale delimiting the Larkin regime parallel to the vortices. The \(a_0^6\) dependence yields^{8,39} an algebraic decay of j_{c}(B) ∝ B^{−3}. As shown in Fig. 3b, we do find j_{c}(B) can be described by an algebraic decay for 0.1 T < B < 0.33 T. With values of j_{0} and j_{c} for our sample, Eq. (2) gives l_{ c } ≈ 10a_{0} over this field range. However the observed algebraic decay is slower than the B^{−3} predicted, with a reduced exponent j_{c}(B) ∝ B^{−1.7}.
Perhaps it is not too surprising that no literature model describes our j_{c} data precisely. All of the theoretical and empirical models described^{8,34,35,36,37,38,39} focus on highκ superconductors. Our sample has low κ = 1.3 and a large part of the superconducting phase diagram is occupied by a Meissner regime (Fig. 1). In what follows we concentrate our analysis at high B, away from the Meissner regime.
For most of the mixed state, i.e. from B = 0.10 to 0.33 T at 1.6 K (Fig. 3b), the sample supports a finite critical current, indicating that vortices are pinned and frozen. At B = 0.34 T there is a sharp downturn in j_{c} and it falls rapidly up to B_{c2}. This indicates vortices are depinning as thermal fluctuations take hold just below B_{c2}. Just below the depinning region at B = 0.335 T, a nascent peak in j_{c} can be seen (Fig. 3b inset). This peak effect is less pronounced than in other reports^{40}, which is to be expected given the weak underlying disorder in our sample. The location of the peak effect is consistent with previous transport measurements and magnetometry on niobium and vanadium under neutron irradiation^{41,42,43} and with transport measurements on niobium and Nb—Ta alloys under plastic deformation^{44,45}. These systematic studies all show the same development of the peak effect: with increasing irradiation or deformation, the peak effect emerges first at high fields close to B_{c2} before developing into a larger peak that pushes to lower fields as the density of pinning centres increases^{41,42}. The reverse effect, where the peak effect is reduced and pushed back up to high fields, is also observed when samples are annealed following neutron irradiation^{43}.
Order–disorder line from smallangle neutron scattering
Following the seminal study by Larkin and Ovchinnikov^{2} on the collective pinning of vortex ensembles, we might expect the jump in j_{c} to be associated with a loss of vortex order. Indeed, peak effects have commonly been linked with orderdisorder transitions of vortex lattices in the literature^{23,40,46,47} To test this paradigm, we directly probe the vortex lattice order in our sample using SANS (Fig. 2).
Neutron scattering is sensitive to correlations between pairs of vortices via the structure factor \(S = \mathop {\sum}\nolimits_{j,k} {\kern 1pt} {\mathrm{e}}^{  {\mathrm{i}}{\bf{q}}.\left( {{\bf{r}}_j  {\bf{r}}_k} \right)}\) where r_{ j } is the position of the jth vortex and q is the scattering vector. The measured scattered intensity as a function of q is the convolution of \(\left {h(q)} \right^2S\) with the instrument resolution function, where h(q) is the form factor of a single vortex. For a perfect vortex lattice, the structure factor consists of δfunction Bragg peaks at reciprocal lattice vectors, with the first such vector appearing at \(g = 2\pi \left( {2B{\mathrm{/\Phi }}_0\sqrt 3 } \right)^{\frac{1}{2}}\) in the case of a triangular lattice. Experimentally the Bragg peak intensity is quantified by integrating the measured scattering over three directions in reciprocal space. This is achieved by measuring rocking curves (Fig. 4a), where the sample, field and vortex lattice are rotated together through the Bragg condition. An area on the 2D SANS multidetector encompassing the Bragg spot is then summed and these summed counts, plotted versus rocking angle (Fig. 4a), are fitted to a Gaussian. The resulting integrated intensity I of the first order Bragg peak is shown in Fig. 4b, for T = 1.6 K after fieldcooling. In the vortex glass, rapidly decaying translational order c_{g} is expected that does not support Bragg peaks. Combined with the rapid falloff of the form factor^{48}, this means little, if any, neutron scattering will be discernible from the vortex glass in our SANS experiments.
We see in Fig. 4b that at T = 1.6 K the integrated intensity I(B) begins a downturn before quickly becoming indiscernible from the background at 0.29 T. We may therefore locate the vortex orderdisorder line B_{dis}(T) at 1.6 K, 0.29 T. Similarly we locate B_{dis}(T) from the field dependence of I at two other temperatures (Fig. 5). All three B_{dis}(T) points identified (crosses in circles in Fig. 1) lie well below B_{c2}(T). B_{dis}(T) may also be determined by measuring the scattered intensity as a function of temperature at constant field. In Fig. 6 we show the scattering measured at the peak of the rocking curve upon warming at 0.13 T, starting from a wellordered vortex ensemble at 2 K. These data also demonstrate the vanishing of neutron intensity well below the upper critical field line and confirm that B_{dis}(T) lies deep in the mixed state.
Bragg glass picture from integrated neutron intensity
For a perfect crystalline lattice, integrating the structure factor S yields a factor 1/g at small scattering angles, so the field dependence of I is described by \(\left {h(g)} \right^2{\mathrm{/}}g\). For the Bragg glass picture, on the other hand, the factor^{3} from integrating S depends on whether the SANS instrument resolution s is larger or smaller than the crossover scale between random manifold and Bragg glass regimes, at which displacements are of the order a_{0}. For SANS measurements with the field and vortices aligned roughly parallel to the neutron beam, the width of the rocking curve probes correlations along the direction of the vortices (see Methods). Then if s < l_{A}, where l_{A} is the crossover scale parallel to the vortices, integrating the structure factor in the Bragg glass picture yields a 1/g, i.e. a B^{−1/2} dependence similar to the perfect crystalline case. If s > l_{A}, the Bragg glass picture produces an additional factor B^{−3/2}. This hypothesis was borne out by the I(B) measured on (K,Ba)BiO_{3} in the first experimental report of the Bragg glass^{3}. Similar I(B) Bragg glass dependences have been reported in the electrondoped cuprate Nd_{1.85}Ce_{0.15}CuO_{4} and in underdoped La_{2−x}Sr_{ x }CuO_{4} (x < 0.15)^{49}.
In Fig. 4b we compare the integrated intensity I(B) measured at 1.6 K with the field dependence expected for a perfect crystalline lattice and that expected in the Bragg glass picture. For these measurements, the instrument resolution s ≈ 240a_{0} along the direction of the vortices (see Methods). Up to B ≈ 0.26 T, i.e. before I fallsoff more sharply as B_{dis} is approached, it can be seen that the field dependence in the Bragg glass picture describes the data rather better than for the perfect crystalline case. We deduce that l_{A} < s ≈ 240a_{0} from our experiments. In elastic theory^{8}, length scales along the vortices and length scales in the vortex plane are coupled through the elastic moduli via \(\sqrt {c_{44}{\mathrm{/}}c_{66}}\). Approximate expressions for the tilt modulus c_{44} ≈ BH and for the shear modulus are^{50}
The shear modulus c_{66} softens close to the upper critical field line as vortex cores start to overlap. Deeper in the mixed state, e.g. for fields 0.1 T < B < 0.33 T, we find the calculated aspect ratio \(\sqrt {c_{44}{\mathrm{/}}c_{66}}\) lies in the range from 2 to 30. An upper bound for the crossover scale r_{A} in the plane of the vortices can thus be determined e.g. at 0.23 T, this upper bound is \(s{\mathrm{/}}\sqrt {c_{44}{\mathrm{/}}c_{66}} \approx 30a_0\). In the next section, we see r_{A} can be precisely quantified using a highresolution SANS setup.
Bragg glass regime from reverse Monte Carlo refinement
To gain more detailed information about the Bragg glass and vortex glass phases in the sample, we employ a second experiment geometry in our SANS measurements. The SANS data in Fig. 4 are collected in the first experiment geometry where applied field and vortices are orientated roughly parallel to the incoming neutron beam (Fig. 2a). In the second experiment geometry, the applied field and vortices are orientated perpendicular to the beam (Fig. 2b). In this geometry, a high instrument resolution in the plane of the vortices is achieved (see Methods) and rocking curves, collected by rotating the sample, field and vortex ensemble together through the Bragg condition, probe correlations within the vortex plane, transverse to the reciprocal lattice vector (Fig. 7). Such data (Fig. 7e) are seen to exhibit an algebraic decay with rotation angle ω. This algebraic decay is characteristic of the Bragg glass regime^{11,19}. The observed exponent ≈ −2.8 (Fig. 7e) is roughly consistent with the value ≈ η_{g} − 3 predicted^{11} for the Bragg glass regime where c_{g}(r) decays algebraically \(\propto r^{  \eta _{\mathrm{g}}}\), with η_{g} ≈ 1 (Table 1).
To uncover more information about the vortex correlations, we use the reverse Monte Carlo (RMC) technique to refine the peak shapes of rocking curves collected in the perpendicular field geometry^{19}. Up to 220,000 vortices are simulated on a computer, with their positions modified successively via Monte Carlo updates, until the observed peak shape is reproduced (see Methods). Meaningful refinements require experimental data that span several decades of rotation angle ω. Long data collection times are needed for the tails where the scattering is weak. We measured such datasets at four selected fields and temperatures in the phase diagram (Fig. 7).
Once the simulated rocking curve numerically reproduces the experimentally measured rocking curve (Fig. 7), correlation functions may be calculated from the simulated vortex positions. A simulated vortex ensemble is not unique: there are many possible simulated microstates that can reproduce the experimental peak shape. However, similar correlation functions are observed to result from such microstates^{19}. In Fig. 8 we show typical correlation functions extracted using RMC at each of the four points measured in the phase diagram. Looking first at the three datasets collected at T = 1.6 K and B = 0.13, 0.18 and 0.23 T, we see these show the same qualitative features, namely two distinct regimes in length scale. At small r, the displacement correlation function b(r) is seen to increase algebraically while c_{g}(r) is seen to decay as a stretched exponential. This clearly represents a random manifold regime^{9,10,11} and accordingly here we fit the data to b(r) ∝ r^{2ζ} and c_{g}(r) ∝ exp{−(r/Λ_{g})^{2β}}. The fitted values of roughness exponent ζ, exponential decay exponent β and the effective correlation length Λ_{g} agree well with theoretical predictions (Table 1). The absence of an observable Larkin regime at small r is consistent with the weak disorder of our sample^{11}. Using the above estimate of l_{c} ≈ 10a_{0} from the critical current, the Larkin regime would be expected at inplane length scales below \(r_{\mathrm{c}} \approx l_{\mathrm{c}}{\mathrm{/}}\sqrt {c_{44}{\mathrm{/}}c_{66}} \approx 2a_0\), a value which is too small to be resolvable from the rdependence of correlation functions.
At large r, we identify a Bragg glass regime (Fig. 8). In this asymptotic regime, b(r) ∝ ln r and \(c_{\mathrm{g}}(r) \propto r^{  \eta _{\mathrm{g}}}\), with the fitted η_{g} ≈ 1 (Table 1). The orientational order g_{6}(r) follows an algebraic decay \(\propto r^{  \eta _6}\) through both the random manifold and the Bragg glass regimes. The fitted exponent η_{6} ≈ 0.2 (Table 1) is rather less than the translational exponent η_{g}, reflecting the longer range of bond orientational order compared to translational order. We conclude that a Bragg glass phase is present at fields and temperatures below the orderdisorder transition B_{dis}(T).
Fracturing of the vortex lattice
We turn now to the fourth dataset collected with long counting times in the perpendicular geometry at 0.17 T and 2.7 K, a point which lies close to the orderdisorder transition B_{dis}(T) (c.f. Fig. 1). Here the rocking curve exhibits a distinctly different shape to the other three RMC datasets measured deeper in the Bragg glass phase. Its brow appears broader (Fig. 7d) and its tails seem less algebraic (Fig. 7e). The correlation functions extracted using RMC show a concomitant suppression of the asymptotic Bragg glass regime: the algebraic decay at large r in c_{g}(r) is no longer visible (Fig. 8c). Only a stretched exponential decay remains, with fitted exponents indicative of the random manifold regime (Table 1). b(r) also shows the sublinear growth expected in this regime.
There is more intriguing behaviour at large r. Here, instead of the slow logarithmic growth that would signal a Bragg glass, b(r) is seen to saturate at ≈ 30a_{0} (Fig. 8a). This suggests the vortex ensemble is fracturing into domains, with reasonable positional order being maintained within each domain and large jumps in displacement, with possible locally amorphous regions, at the domain walls. Indeed, a finite crystalline domain of dimension ≈ 30a_{0} would produce a Bragg peak of finite width ≈ 1.6°, which is roughly consistent with the broadening observed in the rocking curve (Fig. 7d). The orientational order g_{6}(r) for this RMC dataset is reduced compared to the other three RMC datasets, but it continues to decay slowly, with a fitted algebraic exponent η_{6} = 0.07. Moreover, g_{6}(r) persists beyond the domain length scale ≈ 30a_{0}, indicating that domains share roughly similar nearest neighbour directions.
The fracturing observed of the Bragg glass is evocative of the prediction of a multidomain glass phase, that should separate the Bragg glass and vortex liquid phases^{47}. There are differences between prediction and experiment, however. The predicted multidomain glass phase should be confined to a thin sliver in the phase diagram coincident with the peak effect^{47}. Here, on the other hand, the fracturing of the ordered phase is observed at much lower fields and temperatures than the peak effect. The predicted multidomain glass also has both orientational and translational order decaying rapidly beyond the domain length scale, but here we see the orientational order g_{6}(r) survives to larger length scales even in the fractured vortex ensemble. Interestingly, qualitatively similar correlation functions were measured by decoration experiments on the highT_{c} layered cuprate Bi_{2}Sr_{2}CaCu_{2}O_{8+x} (BSCCO)^{51}. The formation of domains was proposed to be a nonequilibrium effect due to finite cooling rates^{51}. We have initiated further SANS explorations to clarify this.
Discussion
The peak effect and other features in magnetometry and transport data are frequently assumed to be underpinned by changes in the positional order of the vortex lattice. Under this assumption, conclusions are sometimes drawn as to the nature of vortex phases without directly probing them. Several features can be identified in magnetometry or transport data, including the irreversibility line (H_{irr}), the peak field (H_{pp}) and the onset of the peak effect regime (H_{po}). In the highT_{ c } cuprates, a broad peak in ΔM may also be present at low temperatures and fields deep in the mixed state and is accordingly designated the fishtail effect or second magnetisation peak^{52}. There are reports of both a sharp peak effect close to B_{c2} and a broad second magnetisation peak well below B_{c2} being observed in the same sample^{53,54} indicating that these two effects are distinct. Accordingly, we should add to our list of features the onset field (H_{fo}), the fishtail peak field (H_{fp}) and the field at which the magnetisation shows a kink (H_{fk}).
On the other hand, the route from ordered vortex ensemble to vortex liquid is envisaged to occur in only one or two sharp steps, i.e. a direct melting from Bragg glass to vortex liquid, or an orderdisorder transition to a vortex glass followed by melting to the liquid. Recent scanning tunnelling microscope (STM) experiments on Codoped NbSe_{2} indicate that there may be two vortex glass phases—a hexatic vortex glass and an amorphous vortex glass^{55}—though it is not clear whether the two phases identified are truly distinct. Nonetheless, there are far fewer disordering transitions than there are features in ΔM and j_{c}. It is an open question as to which of these features, if any, should be tied to an underlying orderdisorder transition in the vortex ensemble. The irreversibility line may reasonably be associated with the melting transition^{25}, since a vortex liquid phase cannot ordinarily support a finite critical current. To which feature, on the other hand, should we associate the Bragg glass to vortex glass transition?
To date only a handful of studies have directly probed the order of the vortex ensemble and simultaneously pinpointed features in magnetisation or critical current. The first such study found the SANS intensity disappeared at the irreversibility line in BSCCO^{25}. This occurred at temperatures consistent with estimates of the melting line using the Ginzburg number and the Lindemann criterion, signalling a link between vortex lattice melting and H_{irr}. In addition, the diffracted neutron intensity was found to vanish abruptly with increasing fields at temperatures well below the irreversibility line, with no reported corresponding features in the bulk magnetisation^{25}. A subsequent muon spin rotation study indicated that this vanishing was due to a 3D to 2D crossover, where the pancake vortices in BSCCO, which arise due to its highly anisotropic layered structure, become decoupled between the superconducting layers^{56}.
Subsequent studies have focussed on the quasitwodimensional layered 2HNbSe_{2} system. Here, due to coexisting charge order, the vortex cores are strongly anisotropic in the plane, adopting a sixfold star shape^{57,58}. Magnetic impurities in 2HNbSe_{2} are adorned by bound states with the same sixfold star shape^{59} which, we suggest, may drive the additional transition from hexatic glass to an amorphous vortex glass observed recently in Codoped NbSe_{2} samples^{55}. Interestingly this transition appears to coincide with the peak field H_{pp}(T) in these samples^{55}, indicating that the Bragg glass to hexatic glass transition should lie at lower fields and temperatures, e.g. perhaps at the onset H_{po}(T). This scenario is consistent with a recent SANS study^{6} on clean NbSe_{2} where the SANS intensity all but disappears at H_{po}(T).
Unfortunately the experimental picture is neither so simple nor general. In Fedoped NbSe_{2}, a wellordered vortex lattice can be observed by SANS at fields much higher than H_{pp}, leading to the conclusion that the peak effect is unrelated to a bulk order–disorder transition^{60}. This conclusion is shared by an earlier decoration study on clean and Fedoped NbSe_{2}^{61}. The picture is muddied further by studies on isotropic conventional superconductors, like niobium, vanadium and V_{3}Si, where vortices have the usual line structure. In V_{3}Si^{62}, the diffracted SANS intensity disappears at H_{pp}(T) but in Nb there are conflicting reports: in one SANS study H_{pp}(T) appears to coincide with the loss of inplane positional order^{63} but in another study a clear SANS signal indicating good vortex order is observed above the peak effect^{4}. Together with our observation of a Bragg glass to vortex glass transition lying at much lower fields and temperatures than H_{pp}(T), we are drawn to the inevitable conclusion that the origin of the order–disorder transition and the origin of the peak effect are not a priori the same.
Recent experimental investigations also show that metastability of the vortex configuration and the associated dependences on history affect the vortex order and consequently the perceived position of the order–disorder transition^{4,6,55,62}. Bulk characteristics from transport^{46,62} and magnetic susceptibility^{6} are also similarly affected. Here we note that our data point for B_{dis}(T) at 0.13 T and 3.74 K (Fig. 6) is obtained by warming the sample at constant field, so it is possible that the vortex configuration is superheated at the perceived order–disorder transition temperature of 3.74 K. If this were the case however, the equilibrium order–disorder transition would lie at even lower temperatures than we report here. Our conclusion, that the order–disorder transition and the peak effect are not necessarily related, would abide.
What are the origins of the order–disorder transition and of the peak effect? One possibility is a change in the nature of the underlying pinning such as a crossover from weak collective to strong pinning^{64}. For weak pinning, the pinning force density \(F_{\mathrm{p}} = j_{\mathrm{c}}B = \left[ {f_{\mathrm{p}}^2{\kern 1pt} n_{\mathrm{p}}\left( {\xi {\mathrm{/}}a_0} \right)^2{\mathrm{/}}V_{\mathrm{c}}} \right]^{1/2}\), where f_{p} is the elementary pinning force and n_{p} = 1/ξ^{2}l is the density of pins, \(V_{\mathrm{c}} = l_{\mathrm{c}}r_{\mathrm{c}}^2\) is the correlation volume over which displacements reach the superconducting coherence length ξ following the random force model^{2,64}. Strong and/or single pinning is identified when f_{p} overcomes the Labusch force^{64} \(f_{\mathrm{L}} \approx {\mathrm{\Phi }}_0^2{\mathrm{/}}4\pi \mu _0\lambda ^2 \approx 10^{  11}\) N for our sample. Since our data do not provide a direct measure of l_{c} or r_{c}, we make an overestimate of \(V_{\mathrm{c}} \approx \sqrt {c_{44}{\mathrm{/}}c_{66}} {\kern 1pt} r_{\mathrm{A}}^3\) to yield an upper bound for f_{p}, which is maximal at low inductions, reaching ≈10^{−13} N. Thus throughout the mixed state \(f_{\mathrm{p}} \ll f_{\mathrm{L}}\) and weak collective pinning is effective. There is no change in pinning regime at B_{dis}(T) or at the peak effect in our sample.
We return to the effect of thermal fluctuations. These allow the vortices to ride over the pinning potential and result in a collapse of the critical current. The onset of fluctuations in our sample is marked by the sharp downturn in j_{c} close to the upper critical field. At T = 1.6 K, this depinning of vortices occurs at B = 0.34 T (Fig. 3b). At 0.3 T, the depinning line lies ≈ 140 mK below B_{c2}(T), substantially below the thermally driven vortex lattice melting line, which we recall is 8 mK below B_{c2}(T) from Eq. (1). One can quantify how far a (B, T) point in the phase diagram lies from B_{c2}(T) using the scaled Thouless temperature a_{T} from the lowest Landau level of the GinzburgLandau theory. Thermodynamic melting is expected^{65} at a_{T} = −9.5. Isotherms of constant a_{T} have approximately the same form as the melting line B_{m}(T) from Eq. (1), so we may identify \( a_{\mathrm{T}} \approx 0.43c_{\mathrm{L}}^{  \frac{4}{3}}\), e.g. a_{T} = −9.5 corresponds to a Lindemann number c_{L} ≈ 0.1. The depinning line in our sample corresponds to a_{T} ≈ −60 or c_{L} ≈ 0.02. The peak effect lies just below this line, i.e. on the edge of the regime where thermal fluctuations dominate. The possibility that thermal fluctuations induce the peak effect has been pointed out previously^{66,67}, however this view must be reconciled with the reported observations of wellordered vortex lattices at temperatures and fields above the peak effect^{4,60}. We suggest that thermal fluctuations sufficiently reduce the order parameter Ψ, such that weak underlying pinning is suddenly accommodated by a rapid but local change in the structure of the vortex cores at the peak effect. This instability, localised to the cores, is not significant at larger scales such as λ or a_{0} so lattice order is not necessarily disturbed through the peak effect.
At the order–disorder transition, on the other hand, the role of thermal fluctuations is insignificant. The four data points for B_{dis}(T) (Fig. 1) lie close to the c_{L} = 0.006 or a_{T} = −360 isotherm, i.e. far from the fluctuation dominated regime. Disorder can be incorporated into lowest Landau level theory via random components in the \(\left {\mathrm{\Psi }} \right^2\) term (δT_{ c } pinning)^{65} and in the \(\left {\mathrm{\Psi }} \right^4\) term^{68}, yielding order–disorder lines where the value of a_{T} varies along the line. We do not find these provide sensible fits to our four data points. We do find a sensible fit is provided by the order–disorder line derived for δT_{ c } pinning using a Lindemannlike approach^{23}. In the limit of vanishing thermal fluctuations, i.e. Gi → 0, B_{dis}(T) then takes the form^{23}
D measures the strength of the disorder and is equal to ξ/l_{c} at 0 K in the Larkin model^{23}. We fit this parameter (Fig. 1), taking c_{L} = 0.2 and obtaining D = 0.12, which is a reasonable value for weak pinning. This yields l_{c} ≈ 3 a_{0} at 0 K, consistent with our earlier estimate from j_{c} and with our RMC results. As B_{dis}(T) is approached upon warming (Fig. 6), the SANS intensity falls continuously to zero, indicating that B_{dis}(T) is a thermodynamic phase transition from Bragg glass to vortex glass. The radial width of the Bragg diffraction spot on the 2D SANS detector also increases as B_{dis} is approached (Fig. 4d), signalling a collapsing translational correlation length. We infer that continuous translational symmetry is broken at the Bragg glass to vortex glass transition. It is still a matter of debate, however, as to which symmetry—if any—is broken between the depinned vortex liquid and pinned vortex glass phases. We expect an exciting era in vortex matter physics, where intriguing possibilities such as the vortex glass being no more than a pinned, hexatic liquid^{18} are experimentally explored using increasingly available highquality STM apparatus.
Overall, our data show that the peak effect and similar features in magnetometry or transport data may not a priori be due to a vortex order–disorder transition. SANS provides a direct probe of vortex order and reveals the order–disorder transition B_{dis}(T) in our sample. It is mediated only by the weak underlying disorder, lying deep in the mixed state, far from the regime dominated by thermal fluctuations. A jump in j_{c} around B_{dis}, as might be expected following the theory of Larkin and Ovchinnikov^{2}, cannot be detected in our j_{c} data derived from magnetometry (Fig. 3b). In contrast, these data show a nascent peak effect at high temperatures and fields, where thermal fluctuations become apparent.
Methods
Laboratory characterisation
Bulk magnetic measurements were carried out using a highfield cryogen free measurement system (CFMS) at the DTU Risø Campus. The field was applied parallel to the [111] crystal axis. We used the GoodmanGor’kov relations^{69} to compare the upper critical field B_{c2}(T) and superconducting critical temperature T_{c} of our sample to the values reported by ref.^{32} for varying sample purity. We calculate a mean free path l = 48 nm, impurity parameter α = 0.84, superconducting coherence length ξ_{0} = 26 nm and London penetration depth λ(0) = 35 nm implying κ = 1.3 for our sample.
Neutron scattering
SANS experiments were performed on three instruments: D22 at the Institut LaueLangevin (Fig. 4), NG7 at the NIST Center for Neutron Research (Fig. 6) and, SANSII at the Swiss Spallation Neutron Source (Figs. 5, 7 and 8). In a typical setup on D22, neutrons of wavelength λ = 0.9 nm with spread Δλ/λ = 0.1 were collimated over a 18 m distance, providing a beam of angular spread a = 0.077°. Scattered neutrons were detected using a 2D multidetector placed 18 m behind the sample (Fig. 2). NG7 and D22 are at reactor sources where the neutron flux at the sample position is constant over experiment time scales. SANSII is at a continuous spallation source with varying neutron flux, so in these experiments multidetector count rates are normalised with a monitor detector situated upstream of the sample. Rather than plotting detector counts/monitor counts, in Fig. 5a and in Fig. 7e the ordinates are scaled to a typical monitor value that was used for measurements containing low or zero vortex signal. When the spallation source is stable, this corresponds to a measurement time of 5 min per rocking angle.
The [111] axis of our vanadium crystal was aligned to within 0.2° of the applied magnetic field direction. Unless otherwise noted, vortex ensembles were prepared by cooling in the desired magnetic field from the normal state, i.e. fieldcooled. Any misalignment between the applied field and the vortex directions due to crystalline anisotropy would have been much smaller than the observed peak widths. In niobium, which has a larger crystalline anisotropy than vanadium, 0.2° of misalignment from [111] would distort the vortex direction by 0.007°^{70}. The edges of the sample were masked from the incident neutrons in view of possible demagnetisation effects.
Two experimental geometries were used in our SANS measurements: (a) the magnetic field was applied roughly parallel to the incident neutron beam (Fig. 2a); (b) the field was applied perpendicular to the beam (Fig. 2b). The parallel geometry was used with a = 0.077° on D22 to survey the field dependence (Fig. 4). This geometry also confirmed the absence of transitions in vortex lattice shape away from the hexagonal symmetry expected for fields along [111]. The perpendicular geometry was used on NG7 with vertical applied field (Fig. 2b) for the temperature dependence (Fig. 6). It was also used on SANSII with horizontal applied field to further map the phase diagram (Fig. 5) and to collect rocking curves with high resolution (a = 0.035°) (Fig. 7) suitable for educing inplane correlations by reverse Monte Carlo refinement. To describe the field dependences of the intensity I integrated over the rocking curve (Figs. 4b and 5c), we used the form factor h calculated for a hexagonal vortex lattice^{48}.
As an initial approximation, the instrument resolution and mosaic spread of the vortex ensemble may be modelled as Gaussian distributions. All widths quoted in this manuscript are fullwidth half maxima. In either experiment geometry, the measured rocking curve width W_{ ω } (Fig. 4a) is given by^{71}
where c is the combined width parallel to the scattering vector: \(c^2{\mathrm{/}}\theta _{\mathrm{B}}^2 = ({\mathrm{\Delta }}\lambda {\mathrm{/}}\lambda )^2 + \gamma ^2\) with θ_{B} the Bragg angle and γ the mosaic spread of the vortex ensemble parallel to the reciprocal lattice vector g. In the parallel geometry, σ probes correlations along the vortices. In the perpendicular geometry, σ probes the direction perpendicular to both the field and to g. The scattering angles are small, e.g. θ_{B} = 0.2° for 0.9 nm neutrons when B = 0.1 T, so c is small in Eq. (5) and the angular spread a of the incoming beam sets the minimum measurable width of the rocking curve.
The radial width W_{r} of the spot on the 2D multidetector measured at the peak of the rocking curve (Fig. 2a) is given by
Equations (5) and (6) may be solved simultaneously to find the unknowns σ and c, and therefore γ. However, due to the smallness of θ_{B}, it is difficult to quantify γ without significant uncertainty. As an alternative, in Fig. 4d we calculate W_{r} assuming γ = 0 and with σ determined from W_{ ω }. The W_{r} values calculated reproduce the measurements for fields up to 0.27 T at 1.6 K (Fig. 4d), indicating that \(\gamma \ll {\mathrm{\Delta }}\lambda {\mathrm{/}}\lambda = 0.1\) in this field range. At higher fields the measured values diverge from the γ = 0 line. This indicates that γ must increase to the order of Δλ/λ = 0.1, i.e. the autocorrelation length parallel to g shrinks to ≈ 3a_{0}.
Reverse Monte Carlo refinement
In reverse Monte Carlo (RMC) refinement, the inplane positions of vortices are simulated on a computer. These positions are recursively modified using a Monte Carlo procedure with cost function \(\chi ^2 = {\sum} {\kern 1pt} \left( {R_{{\mathrm{sim}}}(\omega )  R_{{\mathrm{exp}}}(\omega )} \right)^2{\mathrm{/}}\delta _{{\mathrm{exp}}}(\omega )^2\) where R_{exp}(ω) is the experimentally determined angular dependence of the rocking curve measured in the perpendicular geometry, with corresponding uncertainty δ_{exp}(ω). Simulated rocking curves R_{sim}(ω) are calculated by convolving the elastic structure factor with the experimental resolution before scaling by a factor F, chosen to minimise χ^{2}. Simulated vortex ensembles are chosen to be sufficiently large that finite size effects are insignificant compared to the experimental R_{exp}(ω) widths, varying from 40,000 vortices used for the 0.17 T, 2.7 K dataset (intrinsic simulation width w_{s} = 0.29°) to 220,000 vortices used for the 0.13 T, 1.6 K dataset (w_{s} = 0.12°). Our implementation here extends that used previously for niobium^{19} by incorporating a simulated annealing procedure to assure a global minimum in χ^{2} and to speed up the refinement. Once the minimum in χ^{2} is reached, inplane vortexvortex correlation functions are calculated directly from the simulated ensemble. The simulated ensemble is not unique. For example, it is possible that the measured rocking curve at 0.17 T, 2.7 K (Fig. 7d) could also be reproduced by an ensemble containing large (\(\gg 30a_0\)) domains in which the Bragg glass regime persists, but with average bond angles of neighbouring domains differing to reproduce the observed 3.5° wide distribution in ω. This scenario, for which we note that fracturing of the vortex lattice still occurs, is not accessible in our RMC refinements as the exceptionally large ensemble sizes required lie beyond the computational resources currently available. Similarly, the extra degree of freedom realised by F leads to a gradual decay of correlations with increasing simulation time even after χ^{2} is minimised^{19}, so many different vortex ensembles are generated in each RMC run that all reproduce the shape of the experimental rocking curve. These ensembles are observed to yield the same form for each correlation function^{19}, though the ordinate scale should not be taken too seriously. The ensembles obtained here are all found to be essentially free of dislocations: there is no need to impose minimum nearest neighbour distances or planarity constraints^{19}.
Data availability
The data that support the findings of this study are available from the corresponding author upon request.
References
Larkin, A. I. Effect of inhomogeneities on the structure of the mixed state of superconductors. Sov. Phys. JETP 31, 784–786 (1970).
Larkin, A. I. & Ovchinnikov, Yu. N. Pinning in type II superconductors. J. Low. Temp. Phys. 34, 409–428 (1979).
Klein, T. et al. A Bragg glass phase in the vortex lattice of a type II superconductor. Nature 413, 404–406 (2001).
Ling, X. S. et al. Superheating and supercooling of vortex matter in a Nb single crystal: Direct evidence for a phase transition at the peak effect from neutron diffraction. Phys. Rev. Lett. 86, 712–715 (2001).
Bowell, C. J. et al. Absence of vortex lattice melting in a highpurity Nb superconductor. Phys. Rev. B 82, 144508 (2010).
Marziali Bermúdez, M. et al. Metastability and hysteretic vortex pinning near the orderdisorder transition in NbSe_{2}: Interplay between plastic and elastic energy barriers. Phys. Rev. B 95, 104505 (2017).
Feigel’man, M. V., Geshkenbein, V. B., Larkin, A. I. & Vinokur, V. M. Theory of collective flux creep. Phys. Rev. Lett. 63, 2303–2306 (1989).
Blatter, G., Feigel’man, M. V., Geshkenbein, V. B., Larkin, A. I. & Vinokur, V. M. Vortices in hightemperature superconductors. Rev. Mod. Phys. 66, 1125–1388 (1994).
Bogner, S., Emig, T. & Nattermann, T. Nonuniversal correlations and crossover effects in the Braggglass phase of impure superconductors. Phys. Rev. B 63, 174501 (2001).
Bouchaud, J.P., Mézard, M. & Yedidia, J. S. Variational theory for disordered vortex lattices. Phys. Rev. Lett. 67, 3840–3843 (1991).
Giamarchi, T. & Le Doussal, P. Elastic theory of flux lattices in the presence of weak disorder. Phys. Rev. B 52, 1242–1270 (1995).
Nattermann, T. Scaling approach to pinning: chargedensity waves and giant flux creep in superconductors. Phys. Rev. Lett. 64, 2454–2457 (1990).
Korshunov, S. E. Replica symmetry breaking in vortex glasses. Phys. Rev. B 48, 3969–3975 (1993).
Kierfeld, J. & Vinokur, V. Lindemann criterion and vortex lattice phase transitions in typeII superconductors. Phys. Rev. B 69, 024501 (2004).
Ertas, D. & Nelson, D. R. Irreversibility, mechanical entanglement and thermal melting in superconducting vortex crystals with point impurities. Phys. C. 272, 79–86 (1996).
Giamarchi, T. & Le Doussal, P. Phase diagrams of flux lattices with disorder. Phys. Rev. B 55, 6577–6583 (1997).
Chudnovsky, E. M. Hexatic vortex glass in disordered superconductors. Phys. Rev. B 40, 11355–11357 (1989).
Marchetti, M. C. & Nelson, D. R. Dislocation loops and bondorientational order in the Abrikosov fluxline lattice. Phys. Rev. B 41, 1910–1920 (1990).
Laver, M. et al. Uncovering flux line correlations in superconductors by reverse Monte Carlo refinement of neutron scattering data. Phys. Rev. Lett. 100, 107001 (2008).
Chandra Ganguli, S. et al. Disordering of the vortex lattice through successive destruction of positional and orientational order in a weakly pinned Co_{0.0075}NbSe_{2} single crystal. Sci. Rep. 5, 10613 (2015).
Murray, C. A., Gammel, P. L., Bishop, D. J., Mitzi, D. B. & Kapitulnik, A. Observation of a hexatic vortex glass in flux lattices of the highT _{ c } superconductor Bi_{2.1}Sr_{1.9}Ca_{0.9}Cu_{2}O_{8+δ}. Phys. Rev. Lett. 64, 2312–2315 (1990).
Kim, P., Yao, Z. & Lieber, C. M. Vortex lattice structure in Bi_{2}Sr_{2}CaCu_{2}O_{8+δ} at high temperatures. Phys. Rev. Lett. 77, 5118–5121 (1996).
Mikitik, G. P. & Brandt, E. H. Peak effect, vortexlattice melting line, and orderdisorder transition in conventional and highT _{ c } superconductors. Phys. Rev. B 64, 184514 (2001).
Mikitik, G. P. & Brandt, E. H. Effect of pinning on the vortexlattice melting line in typeII superconductors. Phys. Rev. B 68, 054509 (2003).
Cubitt, R. et al. Direct observation of magnetic flux lattice melting and decomposition in the highT _{ c } superconductor Bi_{2.15}Sr_{1.95}CaCu_{2}O_{8+x}. Nature 365, 407–411 (1993).
Zeldov, E. et al. Thermodynamic observation of firstorder vortexlattice melting transition in Bi_{2}Sr_{2}CaCu_{2}O_{8}. Nature 375, 373–376 (1995).
Schilling, A. et al. Anisotropic latent heat of vortexlattice melting in untwinned YBa_{2}Cu_{3}O_{7−δ}. Phys. Rev. Lett. 78, 4833–4836 (1997).
Lortz, R. et al. Thermal fluctuations and vortex melting in the Nb_{3}Sn superconductor from high resolution specific heat measurements. Phys. Rev. B 74, 104502 (2006).
Kierfeld, J. Topological order in the phase diagram for hightemperature superconductors with point defects. Phys. C. 300, 171–183 (1998).
Kierfeld, J. & Vinokur, V. Dislocations and the critical endpoint of the melting line of vortex line lattices. Phys. Rev. B 61, R14928–R14931 (2000).
Radebaugh, R. & Keesom, P. H. Lowtemperature thermodynamic properties of vanadium. II. Mixed state. Phys. Rev. 149, 217–231 (1966).
Moser, E., Seidl, E. & Weber, H. W. Superconductive properties of vanadium and their impurity dependence. J. Low. Temp. Phys. 49, 585–607 (1982).
Bean, C. P. Magnetization of highfield superconductors. Rev. Mod. Phys. 36, 31–39 (1964).
Campbell, A. M., Evetts, J. E. & DewHughes, D. Pinning of flux vortices in type II superconductors. Philos. Mag. 18, 313–343 (1968).
Fietz, W. A. & Webb, W. W. Hysteresis of superconducting alloys—temperature and field dependence of dislocation pinning in niobium alloys. Phys. Rev. 178, 657–667 (1969).
Kramer, E. J. Scaling laws for flux pinning in hard superconductors. J. Appl. Phys. 44, 1360–1370 (1973).
DewHughes, D. Flux pinning mechanisms in type II superconductors. Philos. Mag. 30, 293–305 (1974).
Eisterer, M. Calculation of the volume pinning force in MgB_{2} superconductors. Phys. Rev. B 77, 144524 (2008).
Feigel’man, M. V. & Vinokur, V. M. Thermal fluctuations of vortex lines, pinning, and creep in highT _{ c } superconductors. Phys. Rev. B 41, 8986–8990 (1990).
Matsushita, T. Flux Pinning in Superconductors (Springer, Berlin Heidelberg, 2007).
Brown, B. S., Blewitt, T. H. & Scott, T. Magnetization measurements on fastneutron irradiated niobium and technetium. Phys. Stat. Sol. (a) 16, 105–113 (1973).
Sekula, S. T. & Kernohan, R. H. Fast neutron damage in superconducting vanadium. In Low Temperature PhysicsLT 13: Volume 3: Superconductivity (eds. Timmerhaus, K. D., O’Sullivan, W. J. & Hammel, E. F.) 217–220 (Springer, Boston, MA, USA, 1974).
Takamura, S. & Okuda, S. The effect of lowtemperature neutron irradiation on the critical current of some superconducting materials. J. Nucl. Mater. 72, 244–248 (1978).
Tedmon, C. S. Jr., Rose, R. M. & Wulff, J. Resistive measurements of structural effects in superconducting niobium. J. Appl. Phys. 36, 829–835 (1965).
Osborne, K. E. & Kramer, E. J. The influence of plastic deformation on the peak effect in a type II superconductor. Philos. Mag. 29, 685–694 (1974).
Henderson, W., Andrei, E. Y., Higgins, M. J. & Bhattacharya, S. Metastability and glassy behavior of a driven fluxline lattice. Phys. Rev. Lett. 77, 2077–2080 (1996).
Menon, G. I. Phase behavior of typeII superconductors with quenched point pinning disorder: A phenomenological proposal. Phys. Rev. B 65, 104527 (2002).
Brandt, E. H. Microscopic theory of clean typeII superconductors in the entire fieldtemperature plane. Phys. Stat. Solidi b 77, 105–119 (1976).
Chang, J. et al. Spin density wave induced disordering of the vortex lattice in superconducting La_{2x}Sr_{ x }CuO_{4}. Phys. Rev. B 85, 134520 (2012).
Brandt, E. H. The fluxline lattice in superconductors. Rep. Prog. Phys. 58, 1465–1594 (1995).
Kim, P., Yao, Z., Bolle, C. A. & Lieber, C. M. Structure of flux line lattices with weak disorder at large length scales. Phys. Rev. B 60, R12589–R12592 (1999).
Daeumling, M., Seuntjens, J. M. & Larbalestier, D. C. Oxygendefect flux pinning, anomalous magnetization and intragrain granularity in YBa_{2}Cu_{3}O_{7δ}. Nature 346, 332–335 (1990).
Sarkar, S. et al. The second magnetization peak and the peak effect phenomenon in the superconductor Ca_{3}Rh_{4}Sn_{13}. Phys. C. 356, 181–191 (2001).
Deligiannis, K. et al. New features in the vortex phase diagram of YBa_{2}Cu_{3}O_{7−δ}. Phys. Rev. Lett. 79, 2121–2124 (1997).
Chandra Ganguli, S. Disorderinduced twostep melting of vortex matter in Cointercalated NbSe_{2} single crystals. Phys. Rev. B 93, 144503 (2006).
Lee, S. L. et al. Evidence for fluxlattice melting and a dimensional crossover in singlecrystal Bi_{2.15}Sr_{1.85}CaCu_{2}O_{8+δ} from muon spin rotation studies. Phys. Rev. Lett. 71, 3862–3865 (1993).
Hess, H. F., Robinson, R. B. & Waszczak, J. V. Vortexcore structure observed with a scanning tunneling microscope. Phys. Rev. Lett. 64, 2711–2714 (1990).
Guillamón, I. et al. Superconducting density of states and vortex cores in 2HNbS_{2}. Phys. Rev. Lett. 101, 166407 (2008).
Ménard, G. C. et al. Coherent longrange magnetic bound states in a superconductor. Nat. Phys. 11, 1013–1016 (2015).
Pautrat, A. et al. Structure of the flux lines lattice in NbSe_{2}: Equilibrium state and influence of the magnetic history. Phys. Rev. B 79, 184511 (2009).
Fasano, Y. et al. Orderdisorder phase transition in NbSe_{2}: Absence of amorphous vortex matter. Phys. Rev. B 66, 020512(R) (2002).
Gapud, A. A., Christen, D. K., Thompson, J. R. & Yethiraj, M. Electrical transport, magnetic, and structural properties of the vortex lattice of V_{3}Si in the vicinity of the peak effect. Phys. Rev. B. 67, 104516 (2003).
Gammel, P. L. et al. Structure and correlations of the flux line lattice in crystalline Nb through the peak effect. Phys. Rev. Lett. 80, 833–836 (1998).
Blatter, G., Geshkenbein, V. G. & Koopmann, J. A. G. Weak to strong pinning crossover. Phys. Rev. Lett. 92, 067009 (2004).
Rosenstein, B. & Li, D. GinzburgLandau theory of type II superconductors in magnetic field. Rev. Mod. Phys. 82, 109–168 (2010).
Mohan, S., Sinha, J., Banerjee, S. S. & Myasoedov, Y. Instabilities in the vortex matter and the peak effect phenomenon. Phys. Rev. Lett. 98, 027003 (2007).
Lortz, R., Musolino, N., Wang, Y., Junod, A. & Toyota, N. Origin of the magnetization peak effect in the Nb_{3}Sn superconductor. Phys. Rev. B 75, 094503 (2007).
Rosenstein, B. & Zhuravlev, V. Quantitative theory of transport in vortex matter of typeII superconductors in the presence of random pinning. Phys. Rev. B 76, 014507 (2007).
Goodman, B. B. The magnetic behaviour of superconductors with negative surface energy. IBM J. Res. Dev. 6, 63–67 (1962).
Christen, D. K. & Thorel, P. Direct observation of the equilibrium misalignment between fluxoids and an applied magnetic field due to anisotropy effects in a typeII superconductor. Phys. Rev. Lett. 42, 191–195 (1979).
Yaron, U. et al. Neutron diffraction studies of flowing and pinned magnetic flux lattices in 2HNbSe_{2}. Phys. Rev. Lett. 73, 2748–2751 (1994).
Acknowledgements
This work was supported by DanScatt. We thank M. R. Eskildsen and E. M. Forgan for helpful comments, and N. H. Andersen for furnishing access to the CFMS. We acknowledge the support of the National Institute of Standards and Technology, U.S. Department of Commerce, in providing neutron research facilities used in this work. J. R. Krzywon, P. D. Butler and S. M. Watson are thanked for assistance on NG7 and with sample environment. This work is partly based on experiments performed at the Swiss spallation neutron source SINQ, Paul Scherrer Institute, Villigen, Switzerland.
Author information
Authors and Affiliations
Contributions
M.L. provided the sample. Magnetisation data were measured by A.B. and R.T.P. and analysed by R.T.P. and M.L. SANS experiments were conducted by M.L. at NG7, S.B., R.T.P. and M.L. at SANSII, and L.P. and M.L. at D22. R.T.P. analysed the SANS data using reverse Monte Carlo refinement, with remaining SANS analysis performed by M.L. The manuscript was written by M.L. with assistance from R.T.P. and contributions from all authors.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
ToftPetersen, R., Abrahamsen, A.B., Balog, S. et al. Decomposing the Bragg glass and the peak effect in a TypeII superconductor. Nat Commun 9, 901 (2018). https://doi.org/10.1038/s4146701803267z
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4146701803267z
This article is cited by

Anisotropic suppression of hyperuniformity of elastic systems in media with planar disorder
Communications Materials (2022)

Second magnetization peak, rhombictosquare Bragg vortex glass transition, and intersecting magnetic hysteresis curves in overdoped BaFe2(As1−xPx)2 single crystals
Scientific Reports (2020)

Unveiling the vortex glass phase in the surface and volume of a typeII superconductor
Communications Physics (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.